Presentation on theme: "ENGINEERING MATERIAL CHAPTER NO.4 CONCRETE"— Presentation transcript:
1ENGINEERING MATERIAL CHAPTER NO.4 CONCRETE INSTRUCTORENGR.MIR WAJAHAT ALIKARDAN INSTITUTE OF HIGHER EDUCATIONDEPARTMENT OF CIVIL ENGINEERING
2INTRODUCTION CONCRETE Concrete is a composite material in which a binding material mixed in water on solidification binds the inert particles of well graded fine and coarse aggregates.Cement and lime are generally used as binding materials, whereas sand cinder is used as fine aggregates and crushed stones, gravel, broken bricks, clinkers are used as coarse aggregates.
3CONCRETEFreshly prepared concrete till it has not yet set is called wet or green concrete. After it has thoroughly set and fully hardened it is called set concrete or just concrete.
4TYPES OF CONCRETE AND ITS USES Concrete are classified into different types:According to binding material used in concrete.According to design of concrete.According to purpose of concrete.
5TYPES OF CONCRETE AND ITS USES CLASSIFICATION ACCORDING TO BINDING MATERIAL:According to binding material used concrete are classified into two types.Cement concrete (2) lime concrete.CEMENT CONCRETEThe concrete consisting of cement, sand and coarse aggregates mixed in a suitable proportions in addition to water is called cement concrete. In this type of concrete cement is used as a binding material, sand as fine aggregates and gravel, crushed stones as coarse aggregates.
6In cement concrete useful proportions of its ingredients are 1 part cement:1-8 part sand:2-16 parts coarse aggregates. USES cement concrete is commonly used in buildings and other important engineering works where strength and durability is of prime importance.
7LIME CONCRETE The concrete consisting of lime, fine aggregates, and coarse aggregates mixed in a suitable proportions with water is called lime concrete. In this type of concrete hydraulic lime is generally used as a binding material, sand and cinder are used as fine aggregates and broken bricks, gravel can be used as coarse aggregates.
8PLACING OF LIME CONCRETE : Placing of concrete shall be completed within three hours of adding water in case of concrete is prepared with hydraulic lime. Concrete should be well cured for a period of atleast 10 days. USES: Lime concrete is generally used for the sake of economy in foundation works, under floors, over roof and where cement is not cheaply and easily available in required quantity.
9TYPES OF CONCRETE AND ITS USES CLASSIFICATION ACCORDING TO DESIGN OF CONCRETEPlain cement concrete.(2) Reinforced cement concrete(RCC).(3) Pre-stressed cement concrete(PCC).PLAIN CEMENT CONCRETEThe cement concrete in which no reinforcement is provided is called plain cement concrete or mass cement concrete.This type of concrete is strong in taking compressive stresses but weak in taking tensile stresses.USES:Plain cement concrete is commonly used in for foundation work and flooring of buildings.
10REINFORCED CEMENT CONCRETE(RCC) The cement concrete in which reinforcement is embedded for taking tensile stress is called reinforced cement concrete.In this type of concrete the steel reinforcement is to be used generally in the form of round bars,6mm to 32mm dia. This concrete is equally strong in taking tensile, compressive and shear stresses. Usual proportions of ingredients in a reinforced concrete are 1part of cement:1-2parts of sand:2-4parts of crushed stones or gravel.USES: RCC is commonly used for construction of slabs, beams, columns, foundation, precast concrete.
13PRE-STRESSED CEMENT CONCRETE (PCC) The cement concrete in which high compressive stresses are artificially induced before their actual use is called pre-stresses cement concrete. in this type of cement concrete, the high compressive stresses are induced by pre-tensioning the reinforcement before placing the concrete, and the reinforcement is released when final setting of the concrete take place. Uses : This concrete can take up high tensile and compressive stresses without development of cracks. The quantity of reinforcement can be considerably reduced by using this concrete.
17TYPES OF CONCRETE AND ITS USES CLASSIFICATION ACCORDING TO PURPOSE According to purpose concrete is classified into following types. a. Vacuum concrete: The cement concrete from which entrained air and excess water is removed after placing it, by suction with the help of vacuum pump is called vacuum concrete. In this concrete the excess water which is added to increase workability but not required for the hydration of cement of concrete is removed by forming vacuum chamber
19b. Air entrained concrete The concrete prepared by mixing aluminum in it is called air entrained ,cellular or aerated concrete. In this concrete bubbles of hydrogen gas are liberated which forms cell and make the concrete cellular. USES: This concrete is used for lining walls and roofs for heat and sound insulation purpose.
21c. Light weight concrete The concrete prepared by using coke breeze, cinder or slag as coarse aggregate is called light weight concrete. The concrete is light in weight and posses heat insulating properties. USES This concrete is used in making precast structural units for partition and wall lining.
22DESCRIPTION OF WORK GRADE OF CONCRETE Concrete in columns, beams 1:1:2 Water retaining structures, Piles, precast work or dense 1:1.5:3 Concrete. RCC beams, slabs, columns 1:2:4 Foundations for buildings, 1:3:6 Mass reinforced works. For mass concrete work. 1:4:8
23WATER CEMENT RATIOIn the preparation of concrete the water cement ratio is very importantFor normal construction the water cement ratio is usually 0.5Adding to much water will reduce the strength of concrete and can cause seggregation.
24WATER CEMENT RATIOFor different ratio of concrete the amount of water for 50kg of cement isConcrete ratio Water quantity1:3: liter1:2: liter1:1.5: liter1:1: liter
25SLUMP TEST SLUMP TEST IS A TEST CONDUCTING BEFORE CONCRETE TO BE USED FOR CASTING. THE PURPOSE OF SLUMP TESTIS TO DETERMINE THE WATER CONTENT IN CONCRETEAND ITS WORKABILITYEQUIPMENT FOR SLUMP TEST:BASE PLATE.TROWEL TO MIX CONCRETE.STEEL TAMPING ROD.SLUMP CONE.RULER.
26SLUMP TEST STEP 1: Fill cone 1/3 full by volume and rod 25 times with 5/8-inch diameterx 24-inch-long hemispherical tip steeltamping rod. (This is aspecification requirementwhich will produce nonstandardresults unless followed exactly.)Distribute rodding evenly over theentire cross section of the sample.
27SLUMP TEST STEP 2: Fill cone 2/3 full by volume. Rod this layer 25 times with rodpenetrating into, but notthrough first layer. Distributerodding evenly over theentire cross section of thelayer.
28SLUMP TEST STEP 3: Remove the excess concrete from the top of the cone, using tamping rodas a screed. Clean overflow from base ofcone.7 Immediately lift cone vertically withslow, even motion. Do not jar the concrete ortilt the cone during this process. Invert thewithdrawn cone, and place next to, but nottouching the slumped concrete. (Perform in5-10 seconds with no lateral or torsionalmotion.)
29SLUMP TEST STEP 4: Lay a straight edge across the top of the slump cone. Measure the amountof slump in inches from the bottom ofthe straight edge to the top of the slumpedconcrete at a point over the originalcenter of the base. The slump operationshall be completed in a maximum elapsedtime of 21/2 minutes. Discard concrete.DO NOT use in any other tests.
30Slump value for different concrete Mass concrete and road work to 5cmOrdinary beams and slabs to 10cmColumns and retaining walls to 12.5cm
31WORKABILITY OF CONCRETE It is the amount of work required to place concrete and to compact it thoroughly.Workability of concrete increases with the addition of water but it reduces the strength that’s why it is not a desirable way of increasing the workability.Use of aggregates which are round and have smooth surfaces increases the workability.
32WORKABILITY OF CONCRETE Workability could also be improved by adding air entraining agent such as vinsol resin or Darex.Use of Lisapole liquid at 30 cubic centimeter per bag of cement improves not only the workability but also the water tightness of concrete.Workability of concrete is better determine by compaction factor test.
34COMPACTION FACTOR TEST The apparatus use for compaction factor test consist of two hoppers Aand B and a cylinder C.The hoppers are providedwith hinged bottom. Thereis a clear distance betweenhopper A and B and cylinderC. the diameter of cylinder Cis 15cm and is of 30cm height.
35COMPACTION FACTOR TEST Cement concrete to be tested is placed in the hopper A and its bottom released. The concrete falling in hopper B achieves some compaction.The bottom of hopper B is now released so that concrete now falls in cylinder C. surplus concrete is removed from the top of cylinder. Concrete in the cylinder is now weighed. Let this weight be W1 .After cleaning the cylinder it is refilled with concrete in layers of 5cm each. Every layer of concrete is thoroughly compacted with an iron rod. Concrete in the cylinder is weighted again. Let this weight be W2 .
36COMPACTION FACTOR TEST The ratio of the two weights is known as compaction factor.Compaction Factor= W1/W2A compaction factor of 0.85 represents a mix of poor workability, 0.92 represents medium and 0.95 represents good workability.
37PLACING OF CONCRETEAfter mixing of concrete it should be placed within 30min of adding of water.It should be quickly transported to the place of lying by means of iron pans manually, in wheel barrows, by pumping or by cranes.In placing, concrete should be laid in thin layers. Each layer being thoroughly consolidated, before the next one is laid.
38PLACING OF CONCRETEConcrete should not be dropped from a height as it would cause segregation of aggregates.In case concrete has more of water or it has been laid in thick layers then on compaction water and fine particles of cement comes at the top forming a layer of weak substance known as laintance
39COMPACTION OF CONCRETE Compaction of concrete is very important in developing qualities like strength, durability, imperviousness by making the concrete dense and free from voids.In case of RCC compaction is done by pinning with an iron rod or even with trowel blade.Excess temping should be avoided as otherwise water, cement and finer particles would come to the surface and results in non uniform concreting.
40COMPACTION OF CONCRETE In case of important and big works, compaction of concrete is done with vibrator.Use of vibrator is best and the most efficient way of compacting concrete. It gives very dense concrete.Care should be taken not to make excessive use of vibrators otherwise the concrete becomes non homogeneous
41CURING OF CONCRETEThe process of keeping concrete wet to enable it to attain full strength is known as curing.The objective of curing is to prevent loss of moisture from concrete due to evaporation or because of any other reasons.Curing should be done for a period of three weeks but not less then 10 days.
42CURING OF CONCRETETo do curing, any one of the following method can be used.The surface of concrete is coated with a layer of bitumen or similar other waterproofing compound which gets into the pores of concrete and prevent loss of water from concrete.Concrete surface is covered with waterproof paper or with a layer of wet sand. It could also be covered with gunny bags.
47QUALITIES OF GOOD CONCRETE STRENGTH: The concrete should be able to withstand the stresses that it is subjected to. It is quite strong in compression but weak in tension.DURABILITY: It should be durable enough to resist the effect of weathering agents.DENSITY: the concrete should be well compacted so that there are no voids or hollows left. It should weigh 3000 kg/cu.m
48QUALITIES OF GOOD CONCRETE WATER TIGHTNESS: when used for construction of water retaining structures such as dams, elevated tanks and water reservoirs then this property of concrete becomes very important. Otherwise the moisture inside the RCC would corrode steel and leakage would start resulting in the ultimate failure of the structure.
49QUALITIES OF GOOD CONCRETE WORKABILITY: It should be easily workable.RESISTANCE TO WEAR AND TEAR: when used in floors and in the construction of roads the concrete should be able to withstand abrasive forces.